#------------------------------------------------------------------------------
#$Date: 2016-03-23 15:16:56 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179320 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/17/4321711.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4321711
loop_
_publ_author_name
'Olivier Tougait'
'James A. Ibers'
_publ_contact_author_address
; Department of Chemistry
  Northwestern University
  2145 Sheridan Rd.
  Evanston, IL 60208-3113, USA
;
_publ_contact_author_email       ibers@chem.nwu.edu
_publ_contact_author_fax         (847)491-2976
_publ_contact_author_name        'James A. Ibers'
_publ_contact_author_phone       (847)491-5449
_publ_section_title
;
 New Series CrLn8Te13Cl (Ln = Sm, Gd, Tb): Pseudo-Misfit-Layer Compounds
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6136
_journal_page_last               6138
_journal_paper_doi               10.1021/ic000817t
_journal_volume                  39
_journal_year                    2000
_chemical_formula_sum            'Cl Cr Gd8 Te13'
_chemical_formula_weight         3004.25
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           36
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_space_group_name_H-M   'C m c 21'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   4.1923(5)
_cell_length_b                   26.464(3)
_cell_length_c                   23.730(3)
_cell_measurement_reflns_used    5712
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      28.746
_cell_measurement_theta_min      2.305
_cell_volume                     2632.7(5)
_computing_cell_refinement       'SMART version 5.054 (Bruker, 1999)'
_computing_data_collection       'SMART version 5.054 (Bruker, 1999)'
_computing_data_reduction        'SAINT-Plus version 6.01 (Bruker, 1999)'
_computing_molecular_graphics    'SHELXTL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXTL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153(2)
_diffrn_measured_fraction_theta_full 0.965
_diffrn_measured_fraction_theta_max 0.965
_diffrn_measurement_device_type  'Brucker Sarmt 1000 CCD'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'standard-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0365
_diffrn_reflns_av_sigmaI/netI    0.0272
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       35
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            15133
_diffrn_reflns_theta_full        28.75
_diffrn_reflns_theta_max         28.75
_diffrn_reflns_theta_min         1.54
_diffrn_standards_decay_%        none
_exptl_absorpt_coefficient_mu    34.449
_exptl_absorpt_correction_T_max  0.762
_exptl_absorpt_correction_T_min  0.076
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed (Sheldrick,1997)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.579
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             4916
_exptl_crystal_size_max          0.324
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.016
_refine_diff_density_max         2.500
_refine_diff_density_min         -2.833
_refine_diff_density_rms         0.726
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.336(10)
_refine_ls_extinction_coef       0.000012(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     141
_refine_ls_number_reflns         3641
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.050
_refine_ls_R_factor_all          0.0243
_refine_ls_R_factor_gt           0.0237
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; calc 
w = 1/[σ²(Fo²)+(0.04Fo²)²]
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0588
_refine_ls_wR_factor_ref         0.0591
_reflns_number_gt                3549
_reflns_number_total             3641
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic000817t_3.cif
_cod_data_source_block           CrGd8Te13Cl
_cod_original_cell_volume        2632.8(5)
_cod_database_code               4321711
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'x, -y, z+1/2'
'-x, y, z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Gd1 Gd 0.0000 0.01787(2) -0.22237(2) 0.00786(12) Uani 1 2 d S . .
Gd2 Gd 0.0000 0.05234(2) -0.55604(2) 0.00766(12) Uani 1 2 d S . .
Gd3 Gd 0.0000 0.10740(2) -0.38437(2) 0.00742(12) Uani 1 2 d S . .
Gd4 Gd 0.0000 0.14797(2) -0.71771(2) 0.00765(12) Uani 1 2 d S . .
Gd5 Gd 0.0000 0.27509(2) -0.40481(2) 0.00752(12) Uani 1 2 d S . .
Gd6 Gd 0.0000 0.44016(2) -0.39743(2) 0.00798(12) Uani 1 2 d S . .
Gd7 Gd 0.0000 0.63207(2) -0.06520(3) 0.00778(11) Uani 1 2 d S . .
Gd8 Gd 0.0000 0.69283(2) -0.23219(2) 0.00737(12) Uani 1 2 d S . .
Te1 Te 0.0000 0.06218(3) 0.00016(3) 0.00753(15) Uani 1 2 d S . .
Te2 Te 0.0000 0.13053(3) -0.16338(3) 0.00713(15) Uani 1 2 d S . .
Te3 Te 0.0000 0.14398(3) -0.85849(3) 0.00726(15) Uani 1 2 d S . .
Te4 Te 0.0000 0.17302(3) -0.49559(3) 0.00935(15) Uani 1 2 d S . .
Te5 Te 0.0000 0.20253(3) -0.00206(3) 0.00786(15) Uani 1 2 d S . .
Te6 Te 0.0000 0.24426(3) -0.62311(3) 0.00891(15) Uani 1 2 d S . .
Te7 Te 0.0000 0.27438(3) -0.26530(3) 0.00690(15) Uani 1 2 d S . .
Te8 Te 0.0000 0.37703(3) -0.11971(3) 0.00776(14) Uani 1 2 d S . .
Te9 Te 0.0000 0.43378(3) -0.25975(3) 0.00772(15) Uani 1 2 d S . .
Te10 Te 0.0000 0.51825(3) -0.12145(3) 0.00702(14) Uani 1 2 d S . .
Te11 Te 0.0000 0.55042(3) -0.45871(3) 0.00744(15) Uani 1 2 d S . .
Te12 Te 0.0000 0.58567(3) -0.28525(3) 0.00787(15) Uani 1 2 d S . .
Te13 Te 0.0000 0.69558(3) -0.36496(3) 0.00789(15) Uani 1 2 d S . .
Cr1 Cr 0.0000 0.29105(7) -0.05909(9) 0.0073(3) Uani 1 2 d S . .
Cl1 Cl 0.0000 -0.00038(10) -0.35262(12) 0.0049(4) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Cl1 Gd1 Te12 67.57(4) . 5_545 ?
Cl1 Gd1 Te12 67.57(4) . 5_445 ?
Te12 Gd1 Te12 83.86(2) 5_545 5_445 ?
Cl1 Gd1 Te10 138.070(15) . 5_545 ?
Te12 Gd1 Te10 85.182(17) 5_545 5_545 ?
Te12 Gd1 Te10 142.77(3) 5_445 5_545 ?
Cl1 Gd1 Te10 138.070(15) . 5_445 ?
Te12 Gd1 Te10 142.77(3) 5_545 5_445 ?
Te12 Gd1 Te10 85.182(17) 5_445 5_445 ?
Te10 Gd1 Te10 82.39(2) 5_545 5_445 ?
Cl1 Gd1 Te9 67.47(4) . 5_445 ?
Te12 Gd1 Te9 135.03(3) 5_545 5_445 ?
Te12 Gd1 Te9 80.057(19) 5_445 5_445 ?
Te10 Gd1 Te9 130.21(3) 5_545 5_445 ?
Te10 Gd1 Te9 77.184(19) 5_445 5_445 ?
Cl1 Gd1 Te9 67.47(4) . 5_545 ?
Te12 Gd1 Te9 80.057(19) 5_545 5_545 ?
Te12 Gd1 Te9 135.03(3) 5_445 5_545 ?
Te10 Gd1 Te9 77.184(19) 5_545 5_545 ?
Te10 Gd1 Te9 130.21(3) 5_445 5_545 ?
Te9 Gd1 Te9 82.37(2) 5_445 5_545 ?
Cl1 Gd1 Te2 124.03(5) . . ?
Te12 Gd1 Te2 71.60(2) 5_545 . ?
Te12 Gd1 Te2 71.60(2) 5_445 . ?
Te10 Gd1 Te2 71.174(19) 5_545 . ?
Te10 Gd1 Te2 71.174(19) 5_445 . ?
Te9 Gd1 Te2 138.696(12) 5_445 . ?
Te9 Gd1 Te2 138.696(12) 5_545 . ?
Te11 Gd2 Te11 84.44(2) 5_545 5_445 ?
Te11 Gd2 Te8 85.337(18) 5_545 6_554 ?
Te11 Gd2 Te8 143.33(3) 5_445 6_554 ?
Te11 Gd2 Te8 143.33(3) 5_545 6_454 ?
Te11 Gd2 Te8 85.337(18) 5_445 6_454 ?
Te8 Gd2 Te8 82.19(2) 6_554 6_454 ?
Te11 Gd2 Te10 141.97(3) 5_545 6_454 ?
Te11 Gd2 Te10 84.817(18) 5_445 6_454 ?
Te8 Gd2 Te10 122.79(3) 6_554 6_454 ?
Te8 Gd2 Te10 71.50(2) 6_454 6_454 ?
Te11 Gd2 Te10 84.817(18) 5_545 6_554 ?
Te11 Gd2 Te10 141.97(3) 5_445 6_554 ?
Te8 Gd2 Te10 71.50(2) 6_554 6_554 ?
Te8 Gd2 Te10 122.79(3) 6_454 6_554 ?
Te10 Gd2 Te10 81.59(2) 6_454 6_554 ?
Te11 Gd2 Te1 71.749(19) 5_545 2_554 ?
Te11 Gd2 Te1 71.749(19) 5_445 2_554 ?
Te8 Gd2 Te1 136.658(14) 6_554 2_554 ?
Te8 Gd2 Te1 136.658(14) 6_454 2_554 ?
Te10 Gd2 Te1 70.238(19) 6_454 2_554 ?
Te10 Gd2 Te1 70.238(19) 6_554 2_554 ?
Te11 Gd2 Te4 73.234(19) 5_545 . ?
Te11 Gd2 Te4 73.234(19) 5_445 . ?
Te8 Gd2 Te4 70.09(2) 6_554 . ?
Te8 Gd2 Te4 70.09(2) 6_454 . ?
Te10 Gd2 Te4 136.836(13) 6_454 . ?
Te10 Gd2 Te4 136.836(13) 6_554 . ?
Te1 Gd2 Te4 132.06(3) 2_554 . ?
Cl1 Gd3 Te11 71.21(4) . 5_445 ?
Cl1 Gd3 Te11 71.21(4) . 5_545 ?
Te11 Gd3 Te11 84.17(2) 5_445 5_545 ?
Cl1 Gd3 Te4 138.14(6) . . ?
Te11 Gd3 Te4 78.10(2) 5_445 . ?
Te11 Gd3 Te4 78.10(2) 5_545 . ?
Cl1 Gd3 Te13 132.42(3) . 5_545 ?
Te11 Gd3 Te13 151.64(3) 5_445 5_545 ?
Te11 Gd3 Te13 89.640(18) 5_545 5_545 ?
Te4 Gd3 Te13 73.55(2) . 5_545 ?
Cl1 Gd3 Te13 132.42(3) . 5_445 ?
Te11 Gd3 Te13 89.640(18) 5_445 5_445 ?
Te11 Gd3 Te13 151.64(3) 5_545 5_445 ?
Te4 Gd3 Te13 73.55(2) . 5_445 ?
Te13 Gd3 Te13 82.78(2) 5_545 5_445 ?
Cl1 Gd3 Te12 68.83(4) . 5_545 ?
Te11 Gd3 Te12 140.03(3) 5_445 5_545 ?
Te11 Gd3 Te12 83.629(19) 5_545 5_545 ?
Te4 Gd3 Te12 135.417(15) . 5_545 ?
Te13 Gd3 Te12 65.97(2) 5_545 5_545 ?
Te13 Gd3 Te12 117.27(3) 5_445 5_545 ?
Cl1 Gd3 Te12 68.83(4) . 5_445 ?
Te11 Gd3 Te12 83.629(19) 5_445 5_445 ?
Te11 Gd3 Te12 140.03(3) 5_545 5_445 ?
Te4 Gd3 Te12 135.417(15) . 5_445 ?
Te13 Gd3 Te12 117.27(3) 5_545 5_445 ?
Te13 Gd3 Te12 65.97(2) 5_445 5_445 ?
Te12 Gd3 Te12 81.76(2) 5_545 5_445 ?
Te7 Gd4 Te7 83.59(2) 6_554 6_454 ?
Te7 Gd4 Te9 140.61(3) 6_554 6_454 ?
Te7 Gd4 Te9 83.821(19) 6_454 6_454 ?
Te7 Gd4 Te9 83.821(19) 6_554 6_554 ?
Te7 Gd4 Te9 140.61(3) 6_454 6_554 ?
Te9 Gd4 Te9 82.69(2) 6_454 6_554 ?
Te7 Gd4 Te8 87.674(17) 6_554 6_554 ?
Te7 Gd4 Te8 146.36(3) 6_454 6_554 ?
Te9 Gd4 Te8 121.35(3) 6_454 6_554 ?
Te9 Gd4 Te8 69.81(2) 6_554 6_554 ?
Te7 Gd4 Te8 146.36(3) 6_554 6_454 ?
Te7 Gd4 Te8 87.674(17) 6_454 6_454 ?
Te9 Gd4 Te8 69.81(2) 6_454 6_454 ?
Te9 Gd4 Te8 121.35(3) 6_554 6_454 ?
Te8 Gd4 Te8 81.85(3) 6_554 6_454 ?
Te7 Gd4 Te3 70.23(2) 6_554 . ?
Te7 Gd4 Te3 70.23(2) 6_454 . ?
Te9 Gd4 Te3 70.38(2) 6_454 . ?
Te9 Gd4 Te3 70.38(2) 6_554 . ?
Te8 Gd4 Te3 136.043(16) 6_554 . ?
Te8 Gd4 Te3 136.043(16) 6_454 . ?
Te7 Gd4 Te6 75.35(2) 6_554 . ?
Te7 Gd4 Te6 75.35(2) 6_454 . ?
Te9 Gd4 Te6 136.001(14) 6_454 . ?
Te9 Gd4 Te6 136.001(14) 6_554 . ?
Te8 Gd4 Te6 71.02(2) 6_554 . ?
Te8 Gd4 Te6 71.02(2) 6_454 . ?
Te3 Gd4 Te6 133.19(3) . . ?
Te13 Gd5 Te13 84.52(2) 5_445 5_545 ?
Te13 Gd5 Te5 84.399(18) 5_445 6_454 ?
Te13 Gd5 Te5 142.26(3) 5_545 6_454 ?
Te13 Gd5 Te5 142.26(3) 5_445 6_554 ?
Te13 Gd5 Te5 84.399(18) 5_545 6_554 ?
Te5 Gd5 Te5 82.68(2) 6_454 6_554 ?
Te13 Gd5 Te3 142.19(3) 5_445 6 ?
Te13 Gd5 Te3 84.655(19) 5_545 6 ?
Te5 Gd5 Te3 123.98(3) 6_454 6 ?
Te5 Gd5 Te3 72.03(2) 6_554 6 ?
Te13 Gd5 Te3 84.655(19) 5_445 6_455 ?
Te13 Gd5 Te3 142.19(3) 5_545 6_455 ?
Te5 Gd5 Te3 72.03(2) 6_454 6_455 ?
Te5 Gd5 Te3 123.98(3) 6_554 6_455 ?
Te3 Gd5 Te3 82.09(2) 6 6_455 ?
Te13 Gd5 Te7 72.11(2) 5_445 . ?
Te13 Gd5 Te7 72.11(2) 5_545 . ?
Te5 Gd5 Te7 136.742(14) 6_454 . ?
Te5 Gd5 Te7 136.742(14) 6_554 . ?
Te3 Gd5 Te7 70.087(19) 6 . ?
Te3 Gd5 Te7 70.087(19) 6_455 . ?
Te13 Gd5 Te4 70.21(2) 5_445 . ?
Te13 Gd5 Te4 70.21(2) 5_545 . ?
Te5 Gd5 Te4 72.09(2) 6_454 . ?
Te5 Gd5 Te4 72.09(2) 6_554 . ?
Te3 Gd5 Te4 137.673(13) 6 . ?
Te3 Gd5 Te4 137.673(13) 6_455 . ?
Te7 Gd5 Te4 128.25(3) . . ?
Cl1 Gd6 Cl1 95.65(8) 5 5_455 ?
Cl1 Gd6 Te3 139.92(6) 5 6_455 ?
Cl1 Gd6 Te3 78.03(5) 5_455 6_455 ?
Cl1 Gd6 Te3 78.03(5) 5 6 ?
Cl1 Gd6 Te3 139.92(6) 5_455 6 ?
Te3 Gd6 Te3 82.01(2) 6_455 6 ?
Cl1 Gd6 Te1 141.20(6) 5 6_454 ?
Cl1 Gd6 Te1 79.13(5) 5_455 6_454 ?
Te3 Gd6 Te1 77.12(2) 6_455 6_454 ?
Te3 Gd6 Te1 129.35(3) 6 6_454 ?
Cl1 Gd6 Te1 79.13(5) 5 6_554 ?
Cl1 Gd6 Te1 141.20(6) 5_455 6_554 ?
Te3 Gd6 Te1 129.35(3) 6_455 6_554 ?
Te3 Gd6 Te1 77.12(2) 6 6_554 ?
Te1 Gd6 Te1 81.54(2) 6_454 6_554 ?
Cl1 Gd6 Te11 70.72(5) 5 . ?
Cl1 Gd6 Te11 70.72(5) 5_455 . ?
Te3 Gd6 Te11 138.838(12) 6_455 . ?
Te3 Gd6 Te11 138.838(12) 6 . ?
Te1 Gd6 Te11 71.311(19) 6_454 . ?
Te1 Gd6 Te11 71.311(19) 6_554 . ?
Cl1 Gd6 Te9 69.71(6) 5 . ?
Cl1 Gd6 Te9 69.71(6) 5_455 . ?
Te3 Gd6 Te9 71.04(2) 6_455 . ?
Te3 Gd6 Te9 71.04(2) 6 . ?
Te1 Gd6 Te9 139.032(12) 6_454 . ?
Te1 Gd6 Te9 139.032(12) 6_554 . ?
Te11 Gd6 Te9 119.45(3) . . ?
Te2 Gd7 Te2 83.95(2) 5_455 5 ?
Te2 Gd7 Te5 142.99(3) 5_455 5 ?
Te2 Gd7 Te5 85.241(18) 5 5 ?
Te2 Gd7 Te5 85.242(18) 5_455 5_455 ?
Te2 Gd7 Te5 142.99(3) 5 5_455 ?
Te5 Gd7 Te5 82.45(2) 5 5_455 ?
Te2 Gd7 Te1 85.103(18) 5_455 5_455 ?
Te2 Gd7 Te1 142.34(3) 5 5_455 ?
Te5 Gd7 Te1 122.87(3) 5 5_455 ?
Te5 Gd7 Te1 71.25(2) 5_455 5_455 ?
Te2 Gd7 Te1 142.34(3) 5_455 5 ?
Te2 Gd7 Te1 85.103(18) 5 5 ?
Te5 Gd7 Te1 71.25(2) 5 5 ?
Te5 Gd7 Te1 122.87(3) 5_455 5 ?
Te1 Gd7 Te1 81.94(2) 5_455 5 ?
Te2 Gd7 Te10 71.76(2) 5_455 . ?
Te2 Gd7 Te10 71.76(2) 5 . ?
Te5 Gd7 Te10 136.625(14) 5 . ?
Te5 Gd7 Te10 136.625(14) 5_455 . ?
Te1 Gd7 Te10 70.59(2) 5_455 . ?
Te1 Gd7 Te10 70.59(2) 5 . ?
Te2 Gd7 Te6 73.99(2) 5_455 2_565 ?
Te2 Gd7 Te6 73.99(2) 5 2_565 ?
Te5 Gd7 Te6 69.01(2) 5 2_565 ?
Te5 Gd7 Te6 69.01(2) 5_455 2_565 ?
Te1 Gd7 Te6 136.159(14) 5_455 2_565 ?
Te1 Gd7 Te6 136.159(14) 5 2_565 ?
Te10 Gd7 Te6 133.32(3) . 2_565 ?
Te6 Gd8 Te12 146.69(3) 2_565 . ?
Te6 Gd8 Te7 80.62(2) 2_565 5 ?
Te12 Gd8 Te7 122.13(2) . 5 ?
Te6 Gd8 Te7 80.62(2) 2_565 5_455 ?
Te12 Gd8 Te7 122.13(2) . 5_455 ?
Te7 Gd8 Te7 84.77(2) 5 5_455 ?
Te6 Gd8 Te2 81.15(2) 2_565 5_455 ?
Te12 Gd8 Te2 74.34(2) . 5_455 ?
Te7 Gd8 Te2 161.76(3) 5 5_455 ?
Te7 Gd8 Te2 92.635(16) 5_455 5_455 ?
Te6 Gd8 Te2 81.15(2) 2_565 5 ?
Te12 Gd8 Te2 74.34(2) . 5 ?
Te7 Gd8 Te2 92.635(16) 5 5 ?
Te7 Gd8 Te2 161.76(3) 5_455 5 ?
Te2 Gd8 Te2 84.19(2) 5_455 5 ?
Te6 Gd8 Te13 145.93(3) 2_565 . ?
Te12 Gd8 Te13 67.38(2) . . ?
Te7 Gd8 Te13 74.42(2) 5 . ?
Te7 Gd8 Te13 74.42(2) 5_455 . ?
Te2 Gd8 Te13 122.29(2) 5_455 . ?
Te2 Gd8 Te13 122.29(2) 5 . ?
Gd7 Te1 Gd7 81.94(2) 5_545 5_445 ?
Gd7 Te1 Gd6 87.152(16) 5_545 6 ?
Gd7 Te1 Gd6 143.77(3) 5_445 6 ?
Gd7 Te1 Gd6 143.77(3) 5_545 6_455 ?
Gd7 Te1 Gd6 87.152(16) 5_445 6_455 ?
Gd6 Te1 Gd6 81.54(2) 6 6_455 ?
Gd7 Te1 Gd2 109.52(2) 5_545 2 ?
Gd7 Te1 Gd2 109.52(2) 5_445 2 ?
Gd6 Te1 Gd2 106.70(2) 6 2 ?
Gd6 Te1 Gd2 106.69(2) 6_455 2 ?
Gd8 Te2 Gd8 84.19(2) 5_545 5_445 ?
Gd8 Te2 Gd7 86.156(16) 5_545 5_545 ?
Gd8 Te2 Gd7 146.06(3) 5_445 5_545 ?
Gd8 Te2 Gd7 146.06(3) 5_545 5_445 ?
Gd8 Te2 Gd7 86.156(16) 5_445 5_445 ?
Gd7 Te2 Gd7 83.95(2) 5_545 5_445 ?
Gd8 Te2 Gd1 104.79(2) 5_545 . ?
Gd8 Te2 Gd1 104.79(2) 5_445 . ?
Gd7 Te2 Gd1 109.13(2) 5_545 . ?
Gd7 Te2 Gd1 109.13(2) 5_445 . ?
Gd5 Te3 Gd5 82.09(2) 6_554 6_454 ?
Gd5 Te3 Gd6 143.02(3) 6_554 6_454 ?
Gd5 Te3 Gd6 86.399(16) 6_454 6_454 ?
Gd5 Te3 Gd6 86.399(16) 6_554 6_554 ?
Gd5 Te3 Gd6 143.02(3) 6_454 6_554 ?
Gd6 Te3 Gd6 82.01(2) 6_454 6_554 ?
Gd5 Te3 Gd4 108.85(2) 6_554 . ?
Gd5 Te3 Gd4 108.85(2) 6_454 . ?
Gd6 Te3 Gd4 108.13(2) 6_454 . ?
Gd6 Te3 Gd4 108.13(2) 6_554 . ?
Cr1 Te4 Cr1 99.27(7) 6_454 6_554 ?
Cr1 Te4 Gd3 130.36(4) 6_454 . ?
Cr1 Te4 Gd3 130.36(4) 6_554 . ?
Cr1 Te4 Gd5 94.09(5) 6_454 . ?
Cr1 Te4 Gd5 94.09(5) 6_554 . ?
Gd3 Te4 Gd5 84.77(2) . . ?
Cr1 Te4 Gd2 95.21(5) 6_454 . ?
Cr1 Te4 Gd2 95.21(5) 6_554 . ?
Gd3 Te4 Gd2 80.84(2) . . ?
Gd5 Te4 Gd2 165.61(3) . . ?
Cr1 Te5 Gd5 101.66(4) . 6 ?
Cr1 Te5 Gd5 101.66(4) . 6_455 ?
Gd5 Te5 Gd5 82.68(2) 6 6_455 ?
Cr1 Te5 Gd7 105.78(4) . 5_445 ?
Gd5 Te5 Gd7 152.54(3) 6 5_445 ?
Gd5 Te5 Gd7 90.956(15) 6_455 5_445 ?
Cr1 Te5 Gd7 105.78(4) . 5_545 ?
Gd5 Te5 Gd7 90.956(15) 6 5_545 ?
Gd5 Te5 Gd7 152.54(3) 6_455 5_545 ?
Gd7 Te5 Gd7 82.45(2) 5_445 5_545 ?
Cr1 Te6 Cr1 99.21(7) 6_554 6_454 ?
Cr1 Te6 Gd8 130.38(4) 6_554 2_564 ?
Cr1 Te6 Gd8 130.38(4) 6_454 2_564 ?
Cr1 Te6 Gd4 96.32(5) 6_554 . ?
Cr1 Te6 Gd4 96.32(5) 6_454 . ?
Gd8 Te6 Gd4 81.37(3) 2_564 . ?
Cr1 Te6 Gd7 95.70(5) 6_554 2_564 ?
Cr1 Te6 Gd7 95.70(5) 6_454 2_564 ?
Gd8 Te6 Gd7 80.03(2) 2_564 2_564 ?
Gd4 Te6 Gd7 161.40(3) . 2_564 ?
Gd8 Te7 Gd8 84.77(2) 5_445 5_545 ?
Gd8 Te7 Gd4 144.30(3) 5_445 6 ?
Gd8 Te7 Gd4 85.038(17) 5_545 6 ?
Gd8 Te7 Gd4 85.038(17) 5_445 6_455 ?
Gd8 Te7 Gd4 144.30(3) 5_545 6_455 ?
Gd4 Te7 Gd4 83.59(2) 6 6_455 ?
Gd8 Te7 Gd5 104.87(2) 5_445 . ?
Gd8 Te7 Gd5 104.87(2) 5_545 . ?
Gd4 Te7 Gd5 110.81(2) 6 . ?
Gd4 Te7 Gd5 110.81(2) 6_455 . ?
Cr1 Te8 Gd2 104.02(4) . 6 ?
Cr1 Te8 Gd2 104.02(4) . 6_455 ?
Gd2 Te8 Gd2 82.19(2) 6 6_455 ?
Cr1 Te8 Gd4 102.34(4) . 6_455 ?
Gd2 Te8 Gd4 153.64(3) 6 6_455 ?
Gd2 Te8 Gd4 92.002(15) 6_455 6_455 ?
Cr1 Te8 Gd4 102.34(4) . 6 ?
Gd2 Te8 Gd4 92.002(15) 6 6 ?
Gd2 Te8 Gd4 153.64(3) 6_455 6 ?
Gd4 Te8 Gd4 81.85(3) 6_455 6 ?
Gd4 Te9 Gd4 82.69(2) 6_455 6 ?
Gd4 Te9 Gd1 145.49(3) 6_455 5 ?
Gd4 Te9 Gd1 87.364(16) 6 5 ?
Gd4 Te9 Gd1 87.365(16) 6_455 5_455 ?
Gd4 Te9 Gd1 145.49(3) 6 5_455 ?
Gd1 Te9 Gd1 82.37(2) 5 5_455 ?
Gd4 Te9 Gd6 110.43(2) 6_455 . ?
Gd4 Te9 Gd6 110.43(2) 6 . ?
Gd1 Te9 Gd6 104.01(2) 5 . ?
Gd1 Te9 Gd6 104.01(2) 5_455 . ?
Gd1 Te10 Gd1 82.39(2) 5_455 5 ?
Gd1 Te10 Gd2 86.095(15) 5_455 6_455 ?
Gd1 Te10 Gd2 142.42(3) 5 6_455 ?
Gd1 Te10 Gd2 142.42(3) 5_455 6 ?
Gd1 Te10 Gd2 86.095(15) 5 6 ?
Gd2 Te10 Gd2 81.59(2) 6_455 6 ?
Gd1 Te10 Gd7 107.92(2) 5_455 . ?
Gd1 Te10 Gd7 107.92(2) 5 . ?
Gd2 Te10 Gd7 109.66(2) 6_455 . ?
Gd2 Te10 Gd7 109.66(2) 6 . ?
Gd2 Te11 Gd2 84.44(2) 5_455 5 ?
Gd2 Te11 Gd3 149.34(3) 5_455 5 ?
Gd2 Te11 Gd3 87.673(15) 5 5 ?
Gd2 Te11 Gd3 87.673(15) 5_455 5_455 ?
Gd2 Te11 Gd3 149.34(3) 5 5_455 ?
Gd3 Te11 Gd3 84.17(2) 5 5_455 ?
Gd2 Te11 Gd6 110.17(2) 5_455 . ?
Gd2 Te11 Gd6 110.17(2) 5 . ?
Gd3 Te11 Gd6 100.37(2) 5 . ?
Gd3 Te11 Gd6 100.37(2) 5_455 . ?
Gd8 Te12 Gd1 109.26(2) . 5_455 ?
Gd8 Te12 Gd1 109.26(2) . 5 ?
Gd1 Te12 Gd1 83.86(2) 5_455 5 ?
Gd8 Te12 Gd3 97.70(2) . 5_455 ?
Gd1 Te12 Gd3 90.842(15) 5_455 5_455 ?
Gd1 Te12 Gd3 152.80(3) 5 5_455 ?
Gd8 Te12 Gd3 97.70(2) . 5 ?
Gd1 Te12 Gd3 152.80(3) 5_455 5 ?
Gd1 Te12 Gd3 90.842(15) 5 5 ?
Gd3 Te12 Gd3 81.76(2) 5_455 5 ?
Gd5 Te13 Gd5 84.52(2) 5 5_455 ?
Gd5 Te13 Gd8 108.60(2) 5 . ?
Gd5 Te13 Gd8 108.60(2) 5_455 . ?
Gd5 Te13 Gd3 153.82(3) 5 5_455 ?
Gd5 Te13 Gd3 90.467(15) 5_455 5_455 ?
Gd8 Te13 Gd3 97.37(2) . 5_455 ?
Gd5 Te13 Gd3 90.467(16) 5 5 ?
Gd5 Te13 Gd3 153.82(3) 5_455 5 ?
Gd8 Te13 Gd3 97.37(2) . 5 ?
Gd3 Te13 Gd3 82.78(2) 5_455 5 ?
Te8 Cr1 Te5 177.71(10) . . ?
Te8 Cr1 Te4 90.03(5) . 6 ?
Te5 Cr1 Te4 91.45(6) . 6 ?
Te8 Cr1 Te4 90.03(5) . 6_455 ?
Te5 Cr1 Te4 91.45(6) . 6_455 ?
Te4 Cr1 Te4 99.27(7) 6 6_455 ?
Te8 Cr1 Te6 89.54(6) . 6_455 ?
Te5 Cr1 Te6 88.98(5) . 6_455 ?
Te4 Cr1 Te6 179.57(9) 6 6_455 ?
Te4 Cr1 Te6 80.758(18) 6_455 6_455 ?
Te8 Cr1 Te6 89.54(6) . 6 ?
Te5 Cr1 Te6 88.98(5) . 6 ?
Te4 Cr1 Te6 80.758(18) 6 6 ?
Te4 Cr1 Te6 179.57(9) 6_455 6 ?
Te6 Cr1 Te6 99.21(7) 6_455 6 ?
Gd6 Cl1 Gd6 95.65(8) 5_445 5_545 ?
Gd6 Cl1 Gd3 116.22(7) 5_445 . ?
Gd6 Cl1 Gd3 116.22(7) 5_545 . ?
Gd6 Cl1 Gd1 117.22(7) 5_445 . ?
Gd6 Cl1 Gd1 117.22(7) 5_545 . ?
Gd3 Cl1 Gd1 95.91(7) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Gd1 Cl1 3.128(3) . ?
Gd1 Te12 3.1369(7) 5_545 ?
Gd1 Te12 3.1369(7) 5_445 ?
Gd1 Te10 3.1828(8) 5_545 ?
Gd1 Te10 3.1828(8) 5_445 ?
Gd1 Te9 3.1831(7) 5_445 ?
Gd1 Te9 3.1831(7) 5_545 ?
Gd1 Te2 3.2938(10) . ?
Gd2 Te11 3.1194(7) 5_545 ?
Gd2 Te11 3.1194(7) 5_445 ?
Gd2 Te8 3.1891(7) 6_554 ?
Gd2 Te8 3.1891(7) 6_454 ?
Gd2 Te10 3.2083(7) 6_454 ?
Gd2 Te10 3.2083(7) 6_554 ?
Gd2 Te1 3.3112(9) 2_554 ?
Gd2 Te4 3.5010(10) . ?
Gd3 Cl1 2.950(3) . ?
Gd3 Te11 3.1274(7) 5_445 ?
Gd3 Te11 3.1274(7) 5_545 ?
Gd3 Te4 3.1594(10) . ?
Gd3 Te13 3.1704(8) 5_545 ?
Gd3 Te13 3.1704(8) 5_445 ?
Gd3 Te12 3.2027(7) 5_545 ?
Gd3 Te12 3.2027(7) 5_445 ?
Gd4 Te7 3.1452(7) 6_554 ?
Gd4 Te7 3.1452(7) 6_454 ?
Gd4 Te9 3.1731(7) 6_454 ?
Gd4 Te9 3.1731(7) 6_554 ?
Gd4 Te8 3.2000(8) 6_554 ?
Gd4 Te8 3.2000(8) 6_454 ?
Gd4 Te3 3.3422(10) . ?
Gd4 Te6 3.3961(10) . ?
Gd5 Te13 3.1168(7) 5_445 ?
Gd5 Te13 3.1168(7) 5_545 ?
Gd5 Te5 3.1734(8) 6_454 ?
Gd5 Te5 3.1734(8) 6_554 ?
Gd5 Te3 3.1923(7) 6 ?
Gd5 Te3 3.1923(7) 6_455 ?
Gd5 Te7 3.3109(10) . ?
Gd5 Te4 3.4548(10) . ?
Gd6 Cl1 2.8285(18) 5 ?
Gd6 Cl1 2.8285(18) 5_455 ?
Gd6 Te3 3.1947(7) 6_455 ?
Gd6 Te3 3.1947(7) 6 ?
Gd6 Te1 3.2099(8) 6_454 ?
Gd6 Te1 3.2099(8) 6_554 ?
Gd6 Te11 3.2601(10) . ?
Gd6 Te9 3.2717(10) . ?
Gd7 Te2 3.1343(7) 5_455 ?
Gd7 Te2 3.1343(7) 5 ?
Gd7 Te5 3.1806(7) 5 ?
Gd7 Te5 3.1806(7) 5_455 ?
Gd7 Te1 3.1970(8) 5_455 ?
Gd7 Te1 3.1970(8) 5 ?
Gd7 Te10 3.2946(10) . ?
Gd7 Te6 3.5496(10) 2_565 ?
Gd8 Te6 3.0776(10) 2_565 ?
Gd8 Te12 3.1028(10) . ?
Gd8 Te7 3.1094(7) 5 ?
Gd8 Te7 3.1094(7) 5_455 ?
Gd8 Te2 3.1270(7) 5_455 ?
Gd8 Te2 3.1270(7) 5 ?
Gd8 Te13 3.1517(10) . ?
Te1 Gd7 3.1970(8) 5_545 ?
Te1 Gd7 3.1970(8) 5_445 ?
Te1 Gd6 3.2099(8) 6 ?
Te1 Gd6 3.2099(8) 6_455 ?
Te1 Gd2 3.3112(9) 2 ?
Te2 Gd8 3.1270(7) 5_545 ?
Te2 Gd8 3.1270(7) 5_445 ?
Te2 Gd7 3.1343(7) 5_545 ?
Te2 Gd7 3.1343(7) 5_445 ?
Te3 Gd5 3.1923(7) 6_554 ?
Te3 Gd5 3.1923(7) 6_454 ?
Te3 Gd6 3.1947(7) 6_454 ?
Te3 Gd6 3.1947(7) 6_554 ?
Te4 Cr1 2.7511(15) 6_454 ?
Te4 Cr1 2.7511(15) 6_554 ?
Te5 Cr1 2.705(2) . ?
Te5 Gd5 3.1734(8) 6 ?
Te5 Gd5 3.1734(8) 6_455 ?
Te5 Gd7 3.1806(7) 5_445 ?
Te5 Gd7 3.1806(7) 5_545 ?
Te6 Cr1 2.7523(15) 6_554 ?
Te6 Cr1 2.7523(15) 6_454 ?
Te6 Gd8 3.0776(10) 2_564 ?
Te6 Gd7 3.5496(10) 2_564 ?
Te7 Gd8 3.1094(7) 5_445 ?
Te7 Gd8 3.1094(7) 5_545 ?
Te7 Gd4 3.1452(7) 6 ?
Te7 Gd4 3.1452(7) 6_455 ?
Te8 Cr1 2.692(2) . ?
Te8 Gd2 3.1891(7) 6 ?
Te8 Gd2 3.1891(7) 6_455 ?
Te8 Gd4 3.2000(8) 6_455 ?
Te8 Gd4 3.2000(8) 6 ?
Te9 Gd4 3.1731(7) 6_455 ?
Te9 Gd4 3.1731(7) 6 ?
Te9 Gd1 3.1831(7) 5 ?
Te9 Gd1 3.1831(7) 5_455 ?
Te10 Gd1 3.1828(8) 5_455 ?
Te10 Gd1 3.1828(8) 5 ?
Te10 Gd2 3.2083(7) 6_455 ?
Te10 Gd2 3.2083(7) 6 ?
Te11 Gd2 3.1194(7) 5_455 ?
Te11 Gd2 3.1194(7) 5 ?
Te11 Gd3 3.1274(7) 5 ?
Te11 Gd3 3.1274(7) 5_455 ?
Te12 Gd1 3.1369(7) 5_455 ?
Te12 Gd1 3.1369(7) 5 ?
Te12 Gd3 3.2027(7) 5_455 ?
Te12 Gd3 3.2027(7) 5 ?
Te13 Gd5 3.1168(7) 5 ?
Te13 Gd5 3.1168(7) 5_455 ?
Te13 Gd3 3.1704(8) 5_455 ?
Te13 Gd3 3.1704(7) 5 ?
Cr1 Te4 2.7511(15) 6 ?
Cr1 Te4 2.7511(15) 6_455 ?
Cr1 Te6 2.7523(15) 6_455 ?
Cr1 Te6 2.7523(15) 6 ?
Cl1 Gd6 2.8285(18) 5_445 ?
Cl1 Gd6 2.8285(18) 5_545 ?
